Chapter 3 Mesoporous Titanium Oxide Doped with Naphthalene Sul-
3.4 Proton Pulsed Field Gradient
The proton PFG-STE NMR experiments of pure NSF exhibit only a single reso- nance at1Hδ≈4 ppm. This suggests that only one of the resonances which are assigned to hydrogen bonded protons in the 1D spectra shown in figure 3.2a contributes to the diffusion as measured by NMR. This suggests there could be structural differences across the NSF resin which prevents certain protons from participating in diffusion. The diffusion rates measured between 20 °C and 100 °C show constant increase as the temperature rises. This is in con- trast to impedance spectroscopy of NSF where the measured impedance starts to decline when the temperature rises above 50 °C. This suggests that there is a macroscopic breakup of NSF which prevents longer distance proton mobility but at the small distances probed by NMR PFG proton mobility continues to increase. The attenuation of the signal in the PFG-STE experiment is linear and can there- fore be simulated with a single diffusion coefficient. The diffusion coefficients are shown in figure 3.8 which have been simulated using an Arrhenius model to estimate the thermal activation energy to proton diffusion which yielded a value of 31±2 kJ mol−1.
The attenuation curves due to diffusion of mTiO2(NSF)-DEE was mea- sured using STE-PFG NMR of proton while spinning at a MAS frequency of 20 kHz. Magic angle spinning was used as static1H STE-PFG was found to yield insufficient signal due to large losses from T2 relaxation caused by the strong homonuclear dipolar coupling between protons. The longer T2 and narrower resonances available from MAS were absolutely necessary to acquire sufficient signal.
The attenuation curves due to diffusion were measured between 20 and 100 °C which were the physical limits of the probe. The effect of changing the diffusion time, ∆, between 50, 100, 200 and 400 ms was examined. The ex- periment at 20 °C and with a diffusion time of 50 ms could not be acquired as the duration of the gradient pulse to detect the diffusion rate became too long for a viable experiment. Therefore this data point had to be abandoned. In all cases the attenuation in the PFG diffusion experiment is not a straight line and
must therefore be described by a model which incorporates more than one diffu- sion coefficient. The most common circumstance which can yield two diffusion coefficients occurs when the proton diffusion pathway includes two different proton transfers with different activation energies and rate constants. However, this mode predicts that as the diffusion time is increased an averaging of the two diffusion rates will occur as each proton experiences both types of transfers. This effect is not seen in this data. The model which best describes this data is the exchange and diffusion between two regions. The assumptions and mathematical description of this model is found in section 2.10.4. It is shown that under these circumstances the attenuation due to diffusion can be written as follows E(g) = exp −γ2δ2g2∆ D2+ P1D1 γ2δ2g2τ 2P1D1+1 , (3.2)
whereγis the proton gyromagnetic ratio, δis the length of the gradient pulse, g is the maximum strength of the gradient pulse and ∆is the length of time protons diffuse. D2is the diffusion rate in region two, P1D1 is the diffusion rate in region one multiplied by the probability of finding the proton in this region and τ2 is the average time a proton spends in region two. The latter three parameters are used to fit the model to the experimental data.
This model describes attenuation in PFG-STE experiment of a species dif- fusing between two types of sub-regions with different diffusion rates which are randomly distributed in a larger area. More precisely the assumption is that dif- fusion in the first sub-region, D1, is substantially quicker than in the second, D2. Under these conditions it is only possible to extract the slower of two diffusion coefficients, D2. The faster diffusion coefficient, D1, can only be extracted as a product with P1, the probability of finding the proton in the fast diffusing sub- region. However, this does give a lower limit on this diffusion rate as P1being a probability will always be less than 1.
This model of fast and slow diffusing regions is consistent with the obser- vation that protons diffuse primarily between NSF sulfonate moieties with the sulfates on the mTiO2 pore wall providing a bridge between the NSF moieties.
2 8 0 3 0 0 3 2 0 3 4 0 3 6 0 3 8 0 1 0 - 1 2 1 0 - 1 1 1 0 - 1 0 1 0 - 9 4 0 0 m s D 2 P 1D 1 2 0 0 m s D 2 P 1D 1 1 0 0 m s D 2 P 1D 1 5 0 m s D 2 P 1D 1 D if fu s io n /m 2 s -1 T e m p e r a t u r e / K 2 0 4 0 6 0 8 0 1 0 0 T e m p e r a t u r e /°C
Figure 3.7: Proton MAS PFG Arrhenius plot of mTiO2(NSF)-DEE with diffusion
times (∆) of 50 ms (green), 100 ms (blue), 200 ms (red) and 400 ms (black). There spectra were acquired on a Bruker Avance III operating at a1H Larmor frequency of 750.10 MHz using a narrow bore Bruker 3.2 mm HXY probe with an imaging gradient coils spinning at a frequency of 20 kHz.
In this scenario the interaction between NSF and the pore wall is weak in cer- tain regions and thus this bridging cannot occur and proton diffusion is forced to proceed mostly directly between NSF moieties. By contrast there are regions where the NSF is arranged such that there is a strong interaction between it and the pore wall. This allows the pore wall bridging between NSF moieties to occur frequently and assuming this type of proton transfer is faster and leads to a higher proton diffusion rate. This interpretation is also consistent with the observation that the D2 diffusion pathway is less thermally stable than P1D1 as would be expected if the interactions between the mTiO2pore wall and the NSF are weaker and therefore more easily disrupted thermally.
Both the fast P1D1 and slow D2 diffusion rates are shown in figure 3.7 and the data has been simulated using the Arrhenius model. The diffusion rates are shown in table 3.3 and the activation energy calculated using the Arrhenius
Table 3.1: The activation energy calculated using the BPP model from spin lat- tice T1relaxation shown in figure 3.5 as well as the activation energy calculated using an Arrhenius fit of the linewidth of the resonance from conduction pro- tons shown in figures 3.2c, 3.3c and 3.4c. The impedance spectroscopy data was collected by Jonathan Turleybut not the Arrhenius analysis presented here.
Sample mTiO2(NSF)-DEE mTiO2(NSF)-H2O NSF /kJ mol−1 /kJ mol−1 /kJ mol−1 Low temperature BPP T1 27±1 20±1 22±4 High temperature BPP T1 32±5 21±6 20±7 Single BPP T1 16.8±0.9 13.0±0.6 12.3±0.5 Stretched Single BPP T1 11±7 4.8±0.2 6.8±0.4 Linewidth Arrhenius 50±4 49±8 50±2 Impedance Spectroscopy 22±2 11±5 -
model are shown in table 3.2. The activation energies have been calculated for the fast diffusion rate, P1D1, assuming that P1 the probability of finding the proton in the fast diffusing region does not change with the diffusion time and temperature.
The activation energies calculated from the fast diffusion component P1D1 vary between 28±5 to 53±8 kJ mol−1depending on which values for the diffu- sion time,∆, was used during acquisition. Initially, when increasing the diffu- sion time from∆=50 to 100 ms the activation energy increases from 38±5 to 53±8 kJ mol−1before decreasing between 200 and 400 ms to 28±5 kJ mol−1.
Table 3.2: The activation energy of NSF and mTiO2(NSF)-DEE calculated from
PFG MAS experiments performed at temperatures between 20 and 100 °C. This data is shown in figure 3.7 and in table 3.3.
∆ P1D1 D2 D
/ms /kJ mol−1 /kJ mol−1 /kJ mol−1 50 38±5
100 53±8 35±3
200 41±4 35±2 31±2 400 28±5 11±4
Table 3.3:The diffusion coefficients of mTiO2(NSF)-DEE measured by MAS PFG using a STE sequence. The data is shown in figure 3.7
∆ Temperature mTiO2(NSF)-DEE mTiO2(NSF)-DEE
/ms /C D2 /m2s−1 P1D1 /m2s−1 50 20 40 2.29±0.02×10−11 5.43±0.3×10−11 60 4.50±0.05×10−11 1.87±0.1×10−10 80 4.03±0.06×10−11 3.10±0.2×10−10 100 3.16±0.06×10−11 5.31±0.5×10−10 100 20 6.7±0.2×10−12 1.28±0.009×10−11 40 2.06±0.03×10−11 1.18±0.05×10−10 60 3.92±0.09×10−11 3.57±0.02×10−10 80 3.23±0.09×10−11 6.69±0.4×10−10 100 3.1±0.2×10−11 1.04±0.2×10−9 200 20 5.8±0.2×10−12 4.33±0.3×10−11 40 1.62±0.05×10−11 1.69±0.07×10−10 60 3.2±0.1×10−11 5.38±0.3×10−10 80 2.35±0.1×10−11 9.25±0.6×10−10 100 2.5±0.3×10−11 1.26±0.2×10−9 400 20 9.6±0.5×10−12 1.26±0.06×10−10 40 1.05±0.05×10−11 2.00±0.08×10−10 60 2.0±0.2×10−11 5.81±0.3×10−10 80 1.3±0.3×10−11 8.77±0.9×10−10 100 1.3±0.5×10−11 1.05±0.2×10−9
This means that the activation energy of mTiO2(NSF)-DEE changes between be- ing just under the activation energy of pure NSF to nearly double as measured by PFG NMR. This large variation in the measurements for mTiO2(NSF)-DEE is likely because the simulation fits P1D1which is the probability of finding the par- ticle in region 1 multiplied with the diffusion rate and not just the diffusion rate, D1. This suggests that P1, the probability of finding a proton in this region, is not constant as the diffusion time∆is changed during the experiments. This is not unexpected as when the regions are sufficiently large that the diffusion time is insufficient for the proton to diffuse through multiple regions subsequently. This leaves the protons predisposed to be found preferentially in one or the other re- gion hence leading to a P1 which changes depending on which diffusion time was used to acquire the data. This limits the information available for the fast component of the diffusion pathway. However, this also increases confidence in the exchange and diffusion model between two regions as alternative models ei- ther predict averaging and merging of D1and D2as∆increase or no dependence on∆for either D1 and D2.
The activation energy of mTiO2(NSF)-DEE calculated for D2 using the Arrhenius model gives 35±3 and 35±2 kJ mol−1 for∆=100 and 200 ms re- spectively. This is very similar to the value calculated for NSF of 31±2 kJ mol−1 which suggests that the primary proton diffusion pathway remains unchanged through NSF. It should be noted that at ∆=400 ms the activation energy cal- culated is significantly lower at 11±4 kJ mol−1. However, this is due to the first diffusion rate measured at 20 °C which is significantly higher than the equiv- alent points measured for ∆ =100 and 200 ms while at 20 °C. Furthermore, the diffusion rates with ∆ = 400 ms at 40 and 60 °C are in agreement with those measured at∆100 and 200 ms. It is therefore reasonable to exclude the activation energy for∆=400 ms.
The activation energies observed using PFG diffusion experiments on NSF and the D2 component of mTiO2(NSF)-DEE are 31±2 and 35±2 kJ mol−1 re- spectively. However, these values do not appear to be in agreement with those measured by T1relaxation or linewidth (T∗2). The T1 activation energy for these samples are lower at between 11±7 and 32±5 kJ mol−1 depending on the
2 8 0 3 0 0 3 2 0 3 4 0 3 6 0 3 8 0 1 0 - 1 2 1 0 - 1 1 1 0 - 1 0 1 0 - 9 1 0 - 8 1 0 - 1 2 1 0 - 1 1 1 0 - 1 0 1 0 - 9 1 0 - 8 D ( m 2 s -1 ) D ( m 2 s -1 ) T e m p e r a t u r e ( K ) 0 2 0 4 0 6 0 8 0 1 0 0 T e m p e r a t u r e ( °C )
Figure 3.8: The Arrhenius plot of NSF (dark green) acquired on two systems a
500 MHz in Warwick (circles) and a 400 MHz in Orleans (squares), mTiO2(NSF) with∆=400 ms (red), water (blue) and Nafion (black) acquired in Warwick (circles), in Orleans (squares) and from literature (triangles).
model used while T∗2activation energy measurements are higher at 50 kJ mol−1. However, both T1 and T∗
2 relaxation are very sensitive to the correlation time of motion but each is sensitive to a different range of correlation times. Given the amorphous nature of NSF there is likely a distribution of energy barriers in the proton diffusion pathway which in turn leads to a distribution of associated correlation frequencies. This would lead to T1and T∗2measurements of different activation depending on their associated correlation time. By contrast measure- ments by PFG diffusion does not depend on the correlation time and therefore is an average of the activation energies.
The above observation further implies a reason for the discrepancy be- tween the activation energy of the PFG diffusion of 35±2 kJ mol−1compared to impedance spectroscopy proton conductivity of 22±2 kJ mol−1. This suggests that there are proton diffusion pathways which are characterised by higher acti- vation energy which do not contribute to overall proton conductivity. The values
for the impedance spectroscopy most closely resemble those of the T1relaxation which suggest that this measurement could be a probe in NSF for the activation energy of the proton conductivity.